Nanotheranostics 2020, Vol. 4
Nanotheranostics 2020; 4(4): 242-255. doi:
Local delivery of insulin/IGF-1 for bone regeneration: carriers,
strategies, and effects Xiaoxuan Zhang1,2*, Helin Xing3*, Feng Qi4,
Hongchen Liu5, Lizeng Gao6 and Xing Wang1,2,5
1. Shanxi Medical University School and Hospital of Stomatology,
Taiyuan 030001, China. 2. Shanxi Province Key Laboratory of Oral
Diseases Prevention and New Materials, Taiyuan 030001 China. 3.
Department of Prosthodontics, Beijing Stomatological Hospital and
School of Stomatology, Capital Medical University, Beijing, 100050,
China. 4. Department of Mechanical and Aerospace Engineering,
University of Missouri, Columbia, MO, USA. 5. Institute of
Stomatology & Oral Maxilla Facial Key Laboratory, Chinese PLA
General Hospital, 28 Fuxing Road, Beijing, 100853, China. 6. CAS
Engineering Laboratory for Nanozyme, Institute of Biophysics,
Chinese Academy of Sciences, Beijing 100101, China.
*These authors contributed equally to this work.
Corresponding authors: Xing Wang, Email: [email protected], Tel:
13934224604; Lizeng Gao, Email: [email protected], Tel:
18752782532; Hongchen Liu, Email: [email protected],
© The author(s). This is an open access article distributed
under the terms of the Creative Commons Attribution License
http://ivyspring.com/terms for full terms and conditions.
Received: 2020.07.18; Accepted: 2020.08.21; Published:
Bone defects caused by trauma, tumor resection, congenital
malformation and infection are still a major challenge for
clinicians. Biomimetic bone materials have attracted more and more
attention in science and industry. Insulin and insulin-like growth
factor-1 (IGF-1) have been increasingly recognized as an inducible
factor for osteogenesis and angiogenesis. Spatiotemporal release of
insulin may serve as the promising strategy. Considering the
successful application of nanoparticles in drug loading, various
insulin delivery systems have been developed, including (poly
(lactic-co-glycolic acid), PLGA), hydroxyapatite (HA), gelatin,
chitosan, alginate, and (γ-glutamic acid)/β-tricalcium phosphate,
γ-PGA/β-TCP). Here, we have reviewed the progress on nanoparticles
carrying insulin/IGF for bone regeneration. In addition, the key
regulatory mechanism of insulin in bone regeneration is also
summarized. The future application strategies and the challenges in
bone regeneration are also discussed.
Key words: Nanoparticles, Insulin, Insulin-like growth factor,
Bone regeneration, Angiogenesis, Osteogenesis
Introduction According to the world health organization,
500,000 bone grafting procedures with a cost greater than $2.5
billion are performed annually in the United States . However,
considerable clinical problems on bone defect are so far
unaddressed, with a remaining group of 10% to 20% of delayed or
nonunion situations . Owing to severe injury or congenital
deformity, osteogenesis insufficiency, rheumatoid arthritis or
osteoporosis, the long and limited self- healing process of bone
grafts cannot fully meet the requirements of timely bone
regeneration sometimes [3-5].
Insulin is a hormone that regulates energy balance and plays an
important role in bone metabolism. Skeletal abnormalities
associated with type I diabetes can be restored after insulin
7]. Clinically, it is often observed that insulin deficiency is
more likely to lead to fracture. In patients with type 2 diabetes
mellitus, the use of insulin treatment significantly increased bone
formation marker procollagen type 1 N-terminal propeptide, which
can reduce the risk of fracture [8, 9]. In vivo studies have shown
that insulin/IGF-1 can promote angiogenesis and provide nutrition
for bone formation [10-12]. Insulin can effectively promote local
skull bone formation by increasing the number of osteoblasts and
osteoid surface area in the mouse skull , and can regulate the
activity of osteoclasts . In recent years, studies have found
that IGF-1 can also affect the growth and development of
osteoblasts, accelerating bone regeneration .
Nanotheranostics 2020, Vol. 4
Figure 1. Summarization of strategies for insulin delivery for
bone regeneration. Various nanoparticles-based delivery systems
have been developed to improve the positive influence of
insulin/IGF-1 on osteogenesis and angiogenesis.
However, the application of insulin in non-
diabetic clinical bone defects has not received much attention,
which may be due to the short life of insulin and the side effects
of too much insulin. For example, the half-life of free insulin is
only 20-30 min [16, 17]. Encapsulated insulin in chitosan
nanoparticles can enhance the absorption of insulin by stem cells
and improve the hypoglycemic effect . This paper reviews the
key regulatory mechanism of insulin in bone regeneration and the
characteristics of different insulin loaded nanoparticles, such as:
(poly (lactic-co- glycolic acid), PLGA), hydroxyapatite (HA),
gelatin, chitosan, alginate, and (γ-glutamic acid)/β-tricalcium
phosphate, γ-PGA/β-TCP) (Figure 1). The application strategies in
bone regeneration are emphasized and the challenges in the future
Potent role of insulin/IGF in bone regeneration
Insulin is derived from pancreatic beta cells, regulating
mammalian cell growth and systemic energy metabolism . Insulin
receptors (IR) are a transmembrane glycoprotein with tyrosine
kinase activity. The binding of insulin with IR causes
auto-phosphorylation of IR [20, 21], activating downstream
phosphoinositide-3-kinase (PI3-K)/Akt and mitogen activated protein
kinase (MAPK) pathways, which affect the differentiation, energy
metabolism and activity of osteocytes [22, 23]. Within a
concentration range, insulin exposure could increase bone
markers, including glucose uptake, alkaline phosphatase (ALP)
production and collagen synthesis. Osteoblasts without IR have
declined osteogenic differentiation, and reduced levels of alkaline
phosphatase and runt-related transcription factor 2 (Runx2) .
IGF is a group of growth- promoting polypeptide substances, whose
secretory cells are widely distributed. IGF-1 has a molecular
structure similar to insulin and possess cross-receptor to activate
the downstream pathway, and IGF-1 can also bind IR and specifically
activate insulin receptor substrate (IRS), a downstream insulin
receptor substrate [24, 25].
Insulin/IGF-1 promote osteogenesis Bone homeostasis is a dynamic
relies on tight interactions between osteoblasts and
osteoclasts. IR exists in osteoblasts and osteoclasts, while IRS
only exists in osteoblasts. IRS is a key factor in signal
transduction of insulin and IGF-1 (Figure 2A). It has a docking
effect with Src homology 2 signal molecules in cells, transferring
the signal through Src homology 3 to Son of Sevenless,
phosphorylating downstream Ras molecules, thereby activating the
extracellular signal-related kinases (ERK1/2) pathway and
regulating the growth, proliferation, and differentiation of
osteoblasts [26, 27]. IRS tyrosine residues phosphorylation
activates PI3-K , which means promotion of the transformation
of phosphatidylinositol-4,5-bisphosphate to
Nanotheranostics 2020, Vol. 4
3,4,5-triphosphate activates downstream AKT and then regulates
the proliferation, survival and energy metabolism of osteoblasts
through mammalian target of rapamycin, BCL-2-antagonist of cell
death, forkhead box O1, and other pathways [28, 29]. IRS in
osteoblasts can regulate the generation of receptor activator of
nuclear factor-kappa B ligand (RANKL), thereby regulating the
differentiation of osteoclasts . Osteoblasts without insulin
receptor substrate 1 cannot generate receptor activator of
NF-kappaB ligand/osteoclast differentiation factor, which is
critical for osteoclast development. The insulin receptor-deficient
mice had been proved to show reduced bone resorption by
osteoclasts, but the bone mass of these mice is still decreased,
indicating that the inhibition of bone formation is stronger than
that of bone resorption .
During bone regeneration, many transcripts must coordinate
various factors to promote osteoblast differentiation, and Runx2
leads early stage differentiation . Runx2 induces osteoblast
differentiation and enhances migration by interacting with PI3K-Akt
signaling . Insulin signaling in osteoblasts plays a role by
promoting the carboxylation of osteocalcin . Osteoblast insulin
receptor (IR) signaling controls osteoblast development and
osteocalcin expression by inhibiting the Runx2 inhibitor Twist2
. Rapamycin complex 1 (mTORC1) is a highly conserved regulator
of cell growth and is one of the most integrated signaling nodes in
all cells. mTORC1 promotes cell growth by
responding to nutrients and growth factors. Insulin has been
found to activate mTORC1 through the PI3K-Akt pathway .
Insulin/IGF-1 promote angiogenesis In mammalian skeletal
formation of endochondral bone coincides with capillary
invasion, suggesting a close relationship between osteogenesis and
angiogenesis . In the osteogenic microenvironment, osteoblasts,
osteoclasts, osteocytes and endothelial progenitor cells are
involved in bone regeneration [34, 35].
Insulin and IGF-1 are important substance for promoting
angiogenesis. Studies have shown that IR in endothelial cells
promotes angiogenesis . Insulin-like growth factor receptors is
also found in the endothelium  (Figure 2B). IGF-1 binding to
insulin-like growth factor receptors can activate downstream IRS
and promote angiogenesis through the MAPK and PI3-K pathways [21,
38, 39]. IGF-1 can activate ERK to promote the formation of
vascular endothelial cells, and the release of nitric oxide by the
PI-3K/Akt pathway to reduce vascular inflammation [40, 41].
Chemokine (C-X-C motif) ligand 9 (Cxcl9) as a direct
anti-regulatory molecule of VEGF signal generated by osteoblasts,
regulating bone angiogenesis and osteogenesis. mTORC1 activates the
expression of Cxcl9 by up-regulating STAT1 and increasing the
binding of STAT1 to the Cxcl9 promoter in osteoblasts ,
suggesting that insulin might promote angiogenesis via Cxcl9.
Figure 2. Insulin / IGF-1 regulates bone regeneration through
MAPK / PI3-K signaling pathway. (A) Insulin / IGF-1 signal
transduction in osteoblasts. (B) IGF-1 promotes angiogenesis by
increasing endothelial cell proliferation.
Nanotheranostics 2020, Vol. 4
Table 1. Characteristics of insulin/IGF-1 nanoparticles
Carrier Synthesis Method Components Drug LE/EE Size Release
behaviour in vitro Effect in bone regeneration Ref PLGA W/O/W
system DCM + PVA + PLGA IGF-1 EE = 78.3% － Initial burst release
h); More than 85% was released within 20 days.
Promote osseointegration of dental implants.
PLGA (W/O/W) system with SPG premix membrane
DCM + PVA + PLGA Insulin LE = 5.4% EE = 60.2%
Initial burst release (51%, 24 h) followed drug release over 5
Bone mineral density (8 week): 0.96 ± 0.06 g/cm3.
LE = 28.27% EE = 67.86%
1.61 μm Initial burst release (29%, 24 h); Sustained release
over 30 days.
Bone mineral density (8 week): 1.10 ± 0.07 g/cm3.
LE = 33.72% EE = 93.29%
21.45 μm Initial lower burst (18%, 24 h); within a long period
up to 2 weeks, the release rate was slow, but then increased in the
Bone mineral density (8 week): 0.86 ± 0.07 g/cm3.
HA Dropwise aqueous
Insulin － < 210 μm － SrHA/insulin promoted stem cell
HA + PEG-DM + DCC + DMAP
IGF-1 LE = 99% 131.3 nm Initial burst release (4g within 24 h);
Sustained release within 28 days.
Increase proliferation of ADSCs on Ti substrates.
O/W emulsion + pDA coating
HA + DCM + PLGA + PVA + DA
IGF-1 － 223.71 μm － Increase proliferation, adhesion, and
osteogenic differentiation of ADSCs.
Gelatin W/W emulsion PEG + Dex-GMA/ gelatin
IGF-1 LE = 5% 30 μm Initial burst release: 20.4 ± 1%, 24 h
release: > 28 days.
Enhance periodontal tissue regeneration.
Gelatin Swell + crosslink OPF + Gelatin microparticles
IGF-1 50-100 μm Initial burst release (30%, 24 h); 1% each day:
Improves the subchondral bone morphology and the interaction
with the surrounding chondral tissue.
Gelatin Heating crosslink OPF + Gelatin + Glutaraldehyde
IGF-1 Loading 100-200 ng: EE = 100%
50-100 μm Initial burst release: (22%, 24 h); Cumulative release
Chitosan Emulsification method
Chitosan + Cottonseed oil + TPP
IGF-1 70.02 ng 50-80 μm 3.31% (14 d) － 
Acetic acid + Chitosan + TPP
IGF-1 168.7 ng 500-700 μm 30.68% (14 d) Enhance pre-osteoblasts
Chitosan W/O emulsion Gelatin + Glyoxal + Chitosan
IGF-1 － － Initial burst release: 48%, 24 h; Sustained release 7
Increase ALP activity of W-20-17 cells.
Alginate Electrospraying method
Sodium alginate chitosan flakes
IGF-1 EE = 40% 296 ± 18 μm 60% within 24 h Promote the
proliferation and differentiation of cementoblasts.
γ-PGA/β-TCP Two-step desolvation
γ-PGA + β-TCP IGF-1 － － 52.86% (12 d) Sequential release of
BMP-2 and IGF-1 significantly promoted the proliferation and
differentiation of MC3T3-E1 cells.
ADSCs: adipose-derived mesenchymal stem cells; ALP: alkaline
phosphatase; BMP-2: bone morphogenetic protein 2; DA: dopamine;
DCM: dichloromethane; DCC: 1,3-dicyclohexylcarbodiimide; Dex-GMA:
dextran-glycidyl methacrylate; DMAP: 4-dimethylaminopyridine; HA:
hydroxyapatite; IGF-1: insulin-like growth factor 1; LE/EE: loading
efficiency/encapsulation efficiency; OPF: oligo(poly(ethylene
glycol) fumarate); pDA: polydopamine; PEG: polyethylene glycol;
PEG-DM: Poly(ethylene glycol) dimethyl ether; PLGA: poly
(lactic-co-glycolic acid); PVA: polyvinyl alcohol; γ-PGA/β-TCP:
(γ-glutamic acid)/β-tricalcium phosphate; SPG: Shirasu porous
glass; SrHA: strontium substitution in HA; TPP: tripolyphosphate;
In summary, vascularization and osteogenesis
are important indicators of bone regeneration .
Insulin/IGF-1 have potent roles in promoting bone regeneration, and
therapeutic delivery of the factors should be beneficial.
Application of insulin/IGF-loaded particles in bone
Nanoparticles is a promising strategy, which has been widely
used to release drugs, maintain local concentration and improve
bioavailability of insulin. Various nanoparticles loaded with
insulin/IGF have been used for bone regeneration, such as those
made of PLGA, HA, chitosan, gelatin, alginate, and γ-PGA/
β-TCP nanoparticles. The preparation method, particle size,
loading efficiency, encapsulation efficiency, and release behavior
of the insulin-loaded nanoparticles are introduced in next part, as
shown in Table 1.
PLGA In the 1970s, polymer particles were firstly
applied involved in the field of biomedicine. Since 1997, the
Food and Drug Administration and European medical institutions
gradually approved the use of PLGA in drug delivery systems .
The degradation rate of PLGA is mainly dependent on the ratio of
glycolic acid to lactic acid monomer . To obtain more detailed
information on accurate
Nanotheranostics 2020, Vol. 4
regulation of the release profile of insulin-loaded particles,
three kinds of uniform-sized insulin microspheres were prepared
using the solvent extraction, solvent evaporation and cosolvent
methods, respectively . It was found that insulin-loaded
microspheres prepared by the solvent evaporation method exhibited a
relatively steady release rate during the first four weeks, which
significantly stimulated the osteogenic differentiation of the stem
cells and peri-implant bone regeneration.
Wang et al.  assessed the IGF-1 PLGA microspheres on bone
healing around implants in type II diabetic rats. The preparation
of PLGA is usually done by W/O/W double emulsion solvent
evaporation process, which can be completed at room temperature.
The average diameter of PLGA microspheres was 1.2525±0.6436 μm. The
surface is smooth. The encapsulation efficiency was 78.3%. The
initial burst release of the IGF-1 microspheres was 55.3% within 2
days, and more than 85% IGF-1 was released within 20 days. The
efficacy of the drug-loaded microspheres was evaluated at 4 and 8
weeks, and the bone-implant contact percentage was found to be
significantly increased in the microspheres group. In this study,
the osteogenic effect was observed by suspending PLGA microspheres
in the blood and then implanting the
implants. The suspended PLGA microspheres may move before
implanting the implants, resulting in uneven distribution. In
addition, the size of nanoparticles also has a great influence on
the release behaviour, but it has not been pointed out. Wang et al.
 investigated the relationship between release kinetics of
insulin and particle size of PLGA nanoparticles in bone
regeneration. In this study, three kinds of insulin-loaded PLGA
particles with narrow size distribution were prepared by Shirasu
porous glass premixed membrane emulsification technology (Figure
3A). The release kinetics showed that the initial release rate of
PLGA microspheres with particle size of 1.61±0.08 μm was about 29%
in the first day, and the remaining insulin ceased to release for
30 days, and accelerated bone defect healing in vivo, compared with
those with sizes of 121.62 nm and 21.45 μm. Wang's experiment
showed that PLGA has the best effect of releasing growth factor to
promote osteogenesis at about 1 um, and in this study, A Shirasu
Glass premixed membrane was specifically used to control the error
to around 0.08, so that the particle size uniformity was improved
and the release stability of the nano-microsphere was increased.
Moreover, smaller particle size error can increase the
repeatability of the experiment and has more potential in
Figure 3. Preparation of insulin-loaded PLGA nanoparticles. (A)
Insulin-loaded PLGA particles were prepared by Shirasu porous glass
premixed membrane emulsification technology. Adapted with
permission from , copyright 2017, American Chemical Society.
(B) Preparation of Cat-HA-PLGA nanoparticles (C) pDA
surface-modified PLGA/HA microspheres were prepared to deliver
Nanotheranostics 2020, Vol. 4
Modification of PLGA Although PLGA nanoparticles are
used in bone tissue engineering for drug delivery, the
hydrophobic nature of PLGA is not conducive to cell adhesion, which
needs further optimization . In order to optimize the effect of
insulin-loaded PLGA on bone regeneration, many methods have been
developed, including surface modification, and combination of PLGA
to different materials .
Using surface modification is a common way to increase the
protein adsorption of PLGA, Choi et al.  studied the
PLGA-grafted hyaluronic acid nanoparticles with surface modified by
catecholamine, which were synthesized by copolymerization method
(Figure 3B). The catechol groups on the surface of nanoparticles
increase the adhesion on the surface of titanium. The
negative-charged hyaluronic acid shell can absorb positive-charged
IGF-1, which improves the loading capacity of IGF-1. The release
rate of growth factor is related to the loading concentration. The
initial burst release is 2% at 200 ng loading in the first 24
hours, and then reaches to 8% within 28 days slowly. In the same
way, polydopamine (pDA) coating on the surface of particles can
induce immobilization of some serum adhesives and adsorption of
some cell types .
Recently, a multifunctional dopamine coating method has been
developed, which only needs to immerse the substrate in alkaline
dopamine solution . Catechol groups of dopamine are oxidized in
an alkaline environment to form pDA layer on organic and inorganic
materials, such as polymers, metal and metal oxides . pDA
surface-modified PLGA/HA microcarriers with a diameter of
223.71±53.39 μm were prepared by Gao et al. , then adipose-
derived mesenchymal stem cells were applied to detect the effect of
pDA @ PLGA/HA/IGF-1 micro-carriers on osteogenic differentiation
(Figure 3C). It was found that the proliferation and the expression
levels of Runx2, osteopontin, and ALP of adipose- derived
mesenchymal stem cells were significantly increased when cultured
on functionalized PLGA/ HA microspheres coated with pDA. The
introduction of HA nanoparticles is of great significance for the
design and preparation of biodegradable PLGA microcarriers. The
addition of HA to PLGA could also improve the stability of PLGA
degradation and provide a certain mechanical strength .
Firstly, due to the improved surface roughness, addition of HA
increases protein adsorption and cell proliferation. Secondly,
surface pre-modification of microcarriers provides an optimization
method for the immobilization of growth factor. Moreover, HA
partially neutralized the local low pH value caused by
degradation of PLGA microspheres, which reduced the effect on the
structural integrity of the transferred IGF-1 [57, 58]. For PLGA
microspheres, the selection of synthetic methods, particle size
control and surface modification can increase the adsorption of
insulin and IGF-1, optimize their release kinetics, and increase
cell adhesion to achieve better osteogenic effect.
HA As the main component of natural bone, HA is
widely used in orthopedics and dentistry to promote
osteogenesis. The advantage of HA in bone is attributed to its
structure and function similar to the mineral composition in bones
and teeth. Due to its nano-structure characteristics and chemical
affinity to molecules, ions and metal, HA is considered as a
delivery system for peptides, proteins, antibiotics, drugs, and
Insulin delivery system based on HA nanospheres has been widely
used in blood glucose regulation [60-62]. Some studies have found
that adding insulin to HA can enhance the effect of HA on
osteogenesis [63, 64]. Lasgorceix et al.  studied the effects
of HA and Si substituted HA granules loaded with insulin on
osteoblasts, but no obvious cell proliferation was observed.
Scudeller et al.  studied the adsorption effect of HA on
insulin. In this study, strontium (SrHA) and zinc (ZnHA) were used
on the surface to replace Ca2+ in HA. Results showed that the
modification of zinc increased the surface area of HA microspheres
and enhanced insulin adsorption capacity of HA microspheres.
However, in vitro cell culture revealed that insulin-loaded SrHA
promoted stromal cell proliferation, whereas insulin-loaded HA and
ZnHA had no such effect, which was related to the fact that the
substitution of strontium did not affect the structure of α helix
of insulin (Figure 4). In the delivery of insulin microspheres, HA
is not easy to degrade, although have good mechanical strength, but
not as good as gel polymer microspheres research widely, but in
other studies, while testing different method for synthesis of
microspheres osteogenesis effect, but no attention to the influence
of insulin microspheres osteogenesis effect is due to the structure
change of the insulin.
Nanoparticles–hydrogel hybrid systems Hydrogels have a wide
range of applications
from tissue engineering to drug delivery. Loading nanoparticles
to produce composite hydrogels that can be used to customize and
extend the mechanical properties of materials has been greatly
developed. Nanoparticles have offered a unique set of
Nanotheranostics 2020, Vol. 4
for drug delivery including high drug loading capacity,
combinatorial delivery, controlled and sustained drug release,
prolonged stability and lifetime, and targeted delivery. To further
enhance therapeutic index, especially for localized application,
nanoparticles have been increasingly combined with hydrogels to
form a hybrid biomaterial system for controlled drug delivery.
Gelatin Gelatin is a commonly used natural polymer,
which is derived from collagen and can be used in under
different conditions of alkalinity, acidity and neutrality. It can
be applied to transfer plasmid DNA, protein and other biological
activity factors, and protect them from loss of bioactivity .
Gelatin particles prepared by different methods have different
degradation characteristics, which will affect the activity of the
carried drugs. Moreover, gelatin easily dissolves rapidly in water,
resulting in increased drug release. Nevertheless, use of a
crosslinking agent is a major factor to maintain the stability of
gelatin particles. Chemical crosslinking is a common solution, but
the presence of residual crosslinkers may lead to toxic side
Using gelatin and dextran and glycidyl methacrylate, Chen et al.
 mixed dextran-glycidyl methacrylate/gelatin solution with
polyethylene glycol aqueous solution to form gelatin microspheres,
then IGF-1 was adsorbed by swelling method (Figure 5A). The
particle size of the microspheres was mostly distributed in 30 μm.
In vivo experiments of animals with periodontal defect, IGF-1
coated with gelatin particles was significantly more effective in
bone formation than IGF-1 isolated in clot. The results
showed that gelatin microspheres had a protective effect on
IGF-1 and were used for drug delivery. Moreover, the use of dextran
as a cross-linking agent can not only avoid the degradation of
gelatin microspheres in IGF-1 solution, but also avoid the harmful
effects caused by residues of chemical cross- linking agent.
To study cartilage repair by IGF-1-loaded nanoparticles, gelatin
particles are also used to make hydrogel complexes of
oligo(poly(ethylene glycol) fumarate) (OPF). Kim et al. 
developed gelatin microparticles composite hydrogel particles by
water oil method. After the adsorption of IGF-1, using
glutaraldehyde crosslinking of macromolecule gel by double the
hydrogel can be carried in cartilage repair two different kinds of
growth factors, and the larger molecular weight reduce the density
of gel, aperture, provide enough space for the cells to grow in,
whether used alone or combined other growth factors, IGF-1
microspheres in the cartilage formation occupied the main role. The
release of IGF-1 from OPF enhances the proliferation of MCF-7 cell
lines and improves the growth of subchondral bone.
Chitosan Chitosan is a kind of amino polysaccharide,
which is obtained by alkaline N-deacetylation of natural
macromolecule chitin . Chitosan and its derivatives have
multiple advantages, such as biodegradability, non-toxic, good
adhesion, renewable resources, low cost, which have been commonly
used in food, medicine and pharmaceutics field, especially in the
development of nano-drug delivery system.
Figure 4. Insulin delivery system based on HA nanoparticles.
Compared to the HA microspheres, the modification of zinc (ZnHA)
enhance insulin adsorption capacity and strontium (SrHA) promotes
stromal cell proliferation.
Nanotheranostics 2020, Vol. 4
Figure 5. Preparation of insulin-loaded nanoparticles using
gelatin, chitosan and alginate. (A) Gelatin Microspheres were
prepared by an aqueous polyethylene glycol /dextran phase
separation method. (B) Chitosan microparticles were prepared by
emulsification and coacervation methods. (C) Insulin loaded
alginate microparticles were prepared by electron spray method.
IGF-1 has been proved to promote the
biomineralization on the surface of chitosan nanoparticles ,
and the use of porous chitosan scaffolds to adsorb IGF-1 can
effectively promote the healing of bone defects . Chitosan
microspheres prepared under different conditions have different
drug release rate. IGF-1-loaded chitosan microspheres can be
prepared by emulsification and coacervation methods  (Figure
5B). The amount of IGF-1 encapsulated by coagulated particles is
about 50% more than that encapsulated by emulsified particles.
After 14 days, only 3.31% of IGF-1 was released from the emulsified
particles, while 30.68% from the coacervation particles, which
indicated that organic solvents had adverse effects on the factors
of the particles in the preparation process. In cell experiments,
chitosan nanoparticles prepared by condensation method was cultured
with osteoblasts. It was found that the nanoparticles enhanced the
proliferation and differentiation of osteoblasts and increased the
expression of osteogenic gene osterix.
When hydrogels with different components are used at the same
time, a dual-transfer system with different factors can be
obtained. Kim et al.  developed and characterized a chitosan
gel/gelatin microspheres dual delivery system. The gelatin
particles were prepared by water-in-oil
emulsification, using glyoxal as a crosslinking agent to improve
the stability of gelatin particles in a water environment. The
obtained particles were encapsulated in chitosan solution to obtain
chitosan/ gelatin particles, and nanoparticles of 50 to 100 µm were
further screened. The microspheres made of chitosan gel and gelatin
can release bone morphogenetic protein-2 and IGF-1 in sequence,
which can significantly improve the ALP activity of w-20-17 cells
compared with that without microspheres. Synergistic growth factors
can reduce the risk of overrelease of single factors and improve
biosafety, but the optimal concentration and degradation properties
of the factors carried by the dual delivery system have not been
studied. Moreover, the above studies only demonstrated the
promotion effect of osteogenesis mineralization at the cellular
level, and the effect and toxicity level in vivo still need to be
Alginate Alginate is a hydrophilic, biodegradable, natural
polysaccharide with low toxicity that forms gel under gentle
condition. Alginate possesses a variety of medical applications
including cell encapsulation, drug stabilization and delivery [76,
77]. Shilpi Goswami  studied the alginate loaded with
Nanotheranostics 2020, Vol. 4
and directly mixed it with alginate solution using calcium
chloride as cross-linking agent. The particle size of the
nanoparticles obtained was not uniform, 40-150 nm. Moreover, it was
found that when the amount of alginate added increased from 1 g to
2 g, hemolytic increased and biosecurity decreased. After loading
insulin with the swelling method, the release was observed to be
close to 60% within 30 min and 100% within 5 h. Duruel et al. 
used electronic spraying method to prepare insulin-loaded alginate
microparticles (Figure 5C). The average diameter of the spherical
alginate particles was 296±18 μm. The encapsulation efficiency was
40%, and the initial release rate was 60% in the first day. In this
study, the longer release time was more appropriate for the slower
cycle of osteogenesis. However, the author believes that in the
sequential release, IGF-1 should be able to release continuously at
the early stage, so alginate particles synthesized in calcium
solution are a suitable choice. After ion exchange under other ions
of microparticles in the medium, IGF-1 will be released by
degradation of microspheres. Alginate particles and chitosan
scaffolds were co-cultured with cementoblast cell line. The results
showed that alginate particles containing IGF-1 promoted the
expression of Runx2 compared with the control group containing
γ-PGA/β-TCP γ-glutamic acid (γ-PGA) has good expansibility
and biocompatibility, and is suitable for clinical applications
such as biogel, drug or gene delivery [80, 81]. Lin et al. 
used a simple and mildly ionic gelation method to make a kind of
nano particle composed of γ-PGA and chitosan, which can effectively
reduce blood glucose level by loading insulin. To moderate pore
size, hardness, and flexibly, γ-PGA is combined with β-tricalcium
phosphate to obtain γ-PGA/TCP nanoparticles for tissue engineering
[83, 84]. Shu et al.  prepared IGF-1 loaded γ-PGA/TCP
particles, and then demonstrated
that the nanoparticles increase the proliferation of MC3T3-E1
cells and ALP activity (Figure 6).
Loading insulin into nanoparticles is a very important way to
achieve desired insulin concentrations locally to improve the
release time, but it is not enough to use nanoparticles alone in
large area of bone defects, because it is difficult to maintain the
morphology of defects. More research on osteogenesis is put into
the combination of biological scaffolds and nano-microspheres. In
the following section, we will highlight the strategy wherein
nanoparticles are combined with scaffolds to improve the osteogenic
effect and provide support for the defect.
Scaffolds based insulin/IGF-1 delivery in bone regeneration
Bone grafts can be classified into allografts bone, autograft
bone, and artificial bone. Autograft is a "gold standard" for
clinical treatment due to its excellent osteogenesis,
osteoinduction, and osteo-conduction , but this method is
limited by the amount of bone supplied at the site of extraction
and causes additional damage to the bone area of the donor.
Allogeneic bone graft can avoid secondary injury in the donor bone
area, but it has the potential risk of infections by viruses .
In recent years, artificial bone materials have become the focus of
research on bone defect repair. Suitable artificial bone
replacement materials should have the following conditions: (1)
simulate the structure of natural bone, providing space for cell
adhesion, angiogenesis and subsequent mineralization; (2) it has
good supporting function; (3) appropriate degradation time to
simulate the reconstruction of natural bone; (4) bio-compatibility:
immune behaviors such as rejection will not be induced; (5) promote
osteogenic differentiation. Current studies include injectable
hydrogel scaffolds, ceramic cement, polymer scaffolds, nanoparticle
loaded scaffolds, etc.
Figure 6. Insulin delivery system based on γ-PGA / TCP
nanoparticles: Preparation and release of γ-PGA / TCP
Nanotheranostics 2020, Vol. 4
HA is the component of bone, so its structure and hardness are
the most similar to natural bone, but the brittleness of HA
materials limits its application in bone tissue engineering [88,
89]. And in the process of bone regeneration, it needs the
continuous absorption of old tissue and the continuous
mineralization of new tissue to carry out a functional
reconstruction. Hydrogels are three-dimensional networks formed by
hydrophilic homopolymers, copolymers or macro-monomers. They swell
in aqueous solution and provide an appropriate microenvironment
similar to extracellular matrix, so as to promote the adhesion,
migration, proliferation and differentiation of chondrocytes.
Hydrogel can be implanted by minimally invasive injection and can
form the desired shape to match irregular defects. Many natural
materials such as chitosan, collagen or gelatin, alginate and
hyaluronic acid can be used to prepare injectable hydrogels.
Although hydrogels can adapt to different shapes of defects, their
mechanical properties are relatively poor . They cannot provide
necessary support when promoting bone formation. Therefore, the
improvement of their mechanical properties needs further study. The
synergistic effect of different components in nano doped biological
scaffolds can solve the defects caused by single materials .
Organo-silane and silk fibroin biopolymers can be assembled into
multifunctional scaffolds. The incorporation of silk fibroin
improves the porosity and mechanical elasticity of aerogel
scaffolds, which can effectively support bone formation .
However, it is not enough only to have good structural
characteristics, but also to induce bone formation. There is a
close relationship between nano materials and bone regeneration,
especially in four main aspects: (1)
Appropriate components in biomaterials can provide continuous
nutrition for bone biomineralization . (2) Nano/microspheres
can carry appropriate growth factors and promote bone
mineralization . (3) Nano/microspheres combined with bone
scaffolds can make up for the mechanical properties of bone
scaffolds, such as adding PLGA microspheres to HA scaffolds .
(4) Nano microspheres can release the growth factors gradually with
the process of osteogenesis, which is more suitable for the process
of osteogenesis .
In bone tissue engineering, artificial materials used to repair
defects are often in the form of scaffolds, among which HA has
mechanical properties similar to those of natural bone. Hydrogel
scaffolds are biocompatible and more plastic, but the scaffolds
alone can only guide bone rather than induce bone regeneration.
Insulin-loaded nanoparticles can improve the mechanical properties
of bone scaffolds and release growth factors in a controlled
manner, making up for the shortcomings of osteogenic scaffolds.
Thus, a composite scaffold of insulin-loaded particles and porous
scaffold may be a preferable strategy (Table 2).
Wang et al.  used the nano-hydroxyapatite/ collagen (nHAC)
as the scaffold of insulin-loaded PLGA particles to repair the
critical defect of rabbit mandible (Figure 7A). At 8 weeks, the new
bone filled and mineralized the defect. nHAC/PLGA composite
scaffolds have good mechanical and structural characteristics in
the repair of large jaw defects, which can maintain the morphology
of the defect site, promote cell adhesion on the scaffolds, and
release insulin at a stable rate to promote the differentiation of
Table 2. Insulin/IGF-1 composited scaffolds in bone
Nanoparticles Scaffold Drug Characterizations of scaffold
Release behaviour of scaffold Effect in bone regeneration Ref
nHAC/PLGA Insulin Nano-nHAC pore size: 127.4 ± 21.1 Initial
burst release (37% within 24 h); Constant release within 10
Enhance proliferation and osteogenesis of BMSCs in vitro;
Restore critical Size bone defect in vivo.
Insulin Micron-nHAC pore size: 122.2 ± 11.4 μm
Initial burst release (23% within 24 h); Sustained release over
the next 30 days.
Insulin 10×Micron-nHAC pore size: 97.2 ± 20.9 μm
Initial burst release (16% within 24 h); Sustained release over
the next 50 days.
Gelatin Dex-GMA/Gelatin IGF-1 Loading 5 ng IGF-1 per mg of
Sustained release during 28 days. Promoting the proliferation,
metabolism and ALP activity of periodic metabolism fibroblasts.
Gelatin OPF IGF-1 Degradation: remained stable over 28 days in
PBS; started to increase after 7 days in collagenase-PBS
Initial released (36.6 ± 8.8%, 4 days) Sustained release during
Enhance cartilage morphology in an osteochondral defect.
Chitosan Chitosan Insulin Scaffolds with 3-mm-height and
5-mm-diameter cylindrical shape
5% insulin initial released: (40%, the first 4 days); 85%
insulin was sustained at 28 days.
Enhance cartilage morphology and the cartilaginous genes
Chitosan IGF-1 Pore size:30–150 μm Porosity of the scaffold:
－ Increased ECM synthesis, cell differentiation and mineralize
ALP: alkaline phosphatase; BMSCs: bone marrow derived
mesenchymal stromal cells; Dex-GMA: dextran-glycidyl methacrylate;
ECM: extracellular matrix; IGF-1: insulin-like growth factor 1;
nHAC: nano-hydroxyapatite/collagen; OPF: oligo(poly(ethylene
glycol) fumarate); PBS: phosphate buffered saline; PLGA: poly
Nanotheranostics 2020, Vol. 4
Figure 7. Preparation of insulin-loaded composite scaffold. (A)
Composite scaffold was prepared using insulin-loaded PLGA
microspheres and nHAC scaffolds. Adapted with permission from ,
copyright 2017, American Chemical Society. (B) Composite scaffold
was prepared using IGF-1 loaded alginate microspheres and chitosan
scaffolds. (C) Preparation of insulin-loaded chitosan scaffold.
The prepared nano-microspheres were placed in
a polymer solution, and then the mixture was placed in the mold
and dried to form a scaffold with a specific shape to carry the
microspheres. As a carrier of growth factor, gelatin particles can
be deposited in the hydrogel to form a solid with fixed shape,
which can provide the release of IGF-1 under the action of
collagenase . The scaffolds synthesized by this method do not
require high temperatures , but the crosslinking agents may be
harmful to organisms. Chen et al.  used IGF-1 loaded
dextran-glycidyl methacrylate/gelatin composite hydrogel scaffolds
instead of single microspheres to obtain more non-toxic composite
scaffolds. Suspended particulate matter in OPF can be used to
obtain integral scaffolds by crosslinking agent without high
temperature, and avoid the decrease in activity caused by thermal
denaturation of bioactive factors . This method has short
crosslinking time, and is easy to obtain bilayer scaffolds.
Duruel et al.  prepared chitosan scaffolds by freeze-drying
method. The internal connection porosity of the scaffold was 80%.
Sodium alginate particles loaded with IGF-1 were integrated into
the scaffold structure, which induced the proliferation
and differentiation of osteoblasts (Figure 7B). Malafaya et al.
 used insulin-loaded chitosan particles to directly form
scaffolds by drying method. Insulin solution and chitosan polymer
were mixed, and then dripped into NaOH by a syringe to obtain
insulin-loaded chitosan particles (Figure 7C). Then the chitosan
particles were placed in the mold and dried at 60 °C to obtain a
scaffold with a specific morphology formed by the materials of the
particles. Chitosan scaffolds release insulin in a dose-dependent
manner to support the adhesion and differentiation of chondrocytes
and the biosynthesis of cartilage matrix. The encapsulation
efficiency of insulin was 87.23%. When the insulin loadings were
5%, the release of chitosan particles was relatively stable.
nHAC scaffolds have high strength and are suitable for the
repair of hard bone defects. The hydrogel was mixed with
nanoparticles, the scaffolds with a more uniform distribution of
nanoparticles were obtained by direct solidification. The
degradation of hydrogel scaffolds is more suitable for the
simultaneous existence of cartilage defects. Moreover, it is easy
to get the desired shape and can obtain double-layer scaffolds with
different growth factors.
Nanotheranostics 2020, Vol. 4
Figure 8. Phases of bone regeneration and the capacity of
insulin-loaded nHAC/PLGA composite scaffolds. Adapted with
permission from , copyright 2017, American Chemical
Conclusion and perspectives To summarize, insulin and IGF-1 have
increasingly recognized as an inducible factor for osteogenesis
and angiogenesis, which is expected to be a preferable drug for
bone regeneration. Nanoparticles have been widely studied in
sustained release, which can provide opportunities for regulating
local insulin concentration and have great potential in bone
regeneration (Figure 8). This review presents the latest advances
of insulin-loaded nanoparticles, including PLGA, HA, gelatin,
chitosan, alginate, and γ-PGA/β-TCP. Information on nano-carriers
introduced in this review is summarized in Table 1. Information on
scaffold introduced in this review is summarized in Table 2. It is
important to note that there remain challenges to be fulfilled. For
example, the loading efficiency remains to be improved. In
addition, the use of insulin-loaded nanoparticles alone is
difficult to provide support and repair of large-scale defects.
Strategies to combine insulin carrying nanoparticles and scaffolds
are needed. In order to control insulin release at the optimal
time, a lot of improvements are undergoing.
In conclusion, bone regeneration is a long-term and complex
process, and local delivery of insulin with various strategies
would certainly promote the process, and produce beneficial effects
in bone regeneration.
Abbreviations ALP: alkaline phosphatase; Cxcl9: chemokine
(C-X-C motif) ligand 9; ERK1/2: extracellular
signal-related kinases; HA: hydroxyapatite; IGF: insulin and
insulin-like growth factor; IGF-1: Insulin-like growth factor 1;
IGFBPs: insulin like growth factor binding proteins; IR: insulin
receptors; IRS: insulin receptor substrate; MAPK: mitogen activated
protein kinase; mTORC1: rapamycin complex 1; nHAC:
nano-hydroxyapatite/collagen; OPF: oligo(poly(ethylene glycol)
fumarate); pDA: polydopamine; PI3-K: phosphoinositide-3-kinase;
PLGA: poly (lactic-co-glycolic acid); RANKL: activator of nuclear
factor kappa B; γ-PGA/β-TCP: (γ-glutamic acid)/β-tricalcium
phosphate; Runx2: runt-related transcription factor 2; SrHA:
strontium substitution in hydroxyapatite; ZnHA: zinc substitution
Acknowledgements This work was supported by National Natural
Science Foundation of China (81801004), Shanxi Province Key
Research and Development Program (201903D321148), Scientific and
Technological Innovation Programs of Higher Education Institutions
in Shanxi (2019L0438, 2020L0209), Graduate Education Innovation
Project of Shanxi Province (2019SY278, 2020SY243) and Shanxi
Medical University School and Hospital of Stomatology (KY201901,
Competing Interests The authors have declared that no
Nanotheranostics 2020, Vol. 4
References 1. Lobb DC, DeGeorge BR Jr, Chhabra AB. Bone graft
concepts and future expectations. J Hand Surg Am. 2019; 44:
497-505.e2. 2. Winkler T, Sass FA, Duda GN, Schmidt-Bleek K. A
review of biomaterials in
bone defect healing, remaining shortcomings and future
opportunities for bone tissue engineering: the unsolved challenge.
Bone Joint Res. 2018; 7: 232-43.
3. Habraken W, Habibovic P, Epple M, Bohner M. Calcium
phosphates in biomedical applications: materials for the future?
Materials Today. 2016; 19: 69-87.
4. Rauch F, Glorieux FH. Osteogenesis imperfecta. Lancet. 2004;
363: 1377-85. 5. Scott DL, Wolfe F, Huizinga TW. Rheumatoid
arthritis. Lancet. 2010; 376:
1094-108. 6. Graham ML, Schuurman HJ. Validity of animal models
of type 1 diabetes, and
strategies to enhance their utility in translational research.
Eur J Pharmacol. 2015; 759: 221-30.
7. Maratova K, Soucek O, Matyskova J, Hlavka Z, Petruzelkova L,
Obermannova B, et al. Muscle functions and bone strength are
impaired in adolescents with type 1 diabetes. Bone. 2018; 106:
8. Nordklint AK, Almdal TP, Vestergaard P, Lundby-Christensen L,
Jørgensen NR, Boesgaard TW, et al. Effect of metformin vs. placebo
in combination with insulin analogues on bone markers P1NP and CTX
in patients with type 2 diabetes mellitus. Calcif Tissue Int. 2020;
9. Vestergaard P, Rejnmark L, Mosekilde L. Relative fracture
risk in patients with diabetes mellitus, and the impact of insulin
and oral antidiabetic medication on relative fracture risk.
Diabetologia. 2005; 48: 1292-9.
10. Hynes B, Kumar AH, O'Sullivan J, Klein Buneker C, Leblond
AL, Weiss S, et al. Potent endothelial progenitor cell-conditioned
media-related anti- apoptotic, cardiotrophic, and pro-angiogenic
effects post-myocardial infarction are mediated by insulin-like
growth factor-1. Eur Heart J. 2013; 34: 782-9.
11. Paglia DN, Wey A, Breitbart EA, Faiwiszewski J, Mehta SK,
Al-Zube L, et al. Effects of local insulin delivery on
subperiosteal angiogenesis and mineralized tissue formation during
fracture healing. J Orthop Res. 2013; 31: 783-91.
12. Rabinovsky ED, Draghia-Akli R. Insulin-like growth factor I
plasmid therapy promotes in vivo angiogenesis. Mol Ther. 2004; 9:
13. Cornish J, Callon KE, Reid IR. Insulin increases
histomorphometric indices of bone formation in vivo. Calcif Tissue
Int. 1996; 59: 492-5.
14. Thomas DM, Udagawa N, Hards DK, Quinn JM, Moseley JM,
Findlay DM, et al. Insulin receptor expression in primary and
cultured osteoclast-like cells. Bone. 1998; 23: 181-6.
15. Xian L, Wu X, Pang L, Lou M, Rosen CJ, Qiu T, et al. Matrix
IGF-1 maintains bone mass by activation of mTOR in mesenchymal stem
cells. Nat Med. 2012; 18: 1095-101.
16. Guler HP, Zapf J, Schmid C, Froesch ER. Insulin-like growth
factors I and II in healthy man. Estimations of half-lives and
production rates. Acta Endocrinol (Copenh). 1989; 121: 753-8.
17. Duan C, Xu Q. Roles of insulin-like growth factor (IGF)
binding proteins in regulating IGF actions. Gen Comp Endocrinol.
2005; 142: 44-52.
18. Li H, Zhang Z, Bao X, Xu G, Yao P. Fatty acid and quaternary
ammonium modified chitosan nanoparticles for insulin delivery.
Colloids Surf B Biointerfaces. 2018; 170: 136-43.
19. Ferron M, Wei J, Yoshizawa T, Del Fattore A, DePinho RA,
Teti A, et al. Insulin signaling in osteoblasts integrates bone
remodeling and energy metabolism. Cell. 2010; 142: 296-308.
20. Fulzele K, Riddle RC, DiGirolamo DJ, Cao X, Wan C, Chen D,
et al. Insulin receptor signaling in osteoblasts regulates
postnatal bone acquisition and body composition. Cell. 2010; 142:
21. Saltiel AR, Kahn CR. Insulin signalling and the regulation
of glucose and lipid metabolism. Nature. 2001; 414: 799-806.
22. Yang J, Zhang X, Wang W, Liu J. Insulin stimulates
osteoblast proliferation and differentiation through ERK and PI3K
in MG-63 cells. Cell Biochem Funct. 2010; 28: 334-41.
23. Ogata N, Chikazu D, Kubota N, Terauchi Y, Tobe K, Azuma Y,
et al. Insulin receptor substrate-1 in osteoblast is indispensable
for maintaining bone turnover. J Clin Invest. 2000; 105:
24. Xuan NT, Hoang NH, Nhung VP, Duong NT, Ha NH, Hai NV.
Regulation of dendritic cell function by insulin/IGF-1/PI3K/Akt
signaling through klotho expression. J Recept Signal Transduct Res.
2017; 37: 297-303.
25. Denley A, Carroll JM, Brierley GV, Cosgrove L, Wallace J,
Forbes B, et al. Differential activation of insulin receptor
substrates 1 and 2 by insulin-like growth factor-activated insulin
receptors. Mol Cell Biol. 2007; 27: 3569-77.
26. Lowenstein EJ, Daly RJ, Batzer AG, Li W, Margolis B, Lammers
R, et al. The SH2 and SH3 domain-containing protein GRB2 links
receptor tyrosine kinases to ras signaling. Cell. 1992; 70:
27. Fritsche L, Neukamm SS, Lehmann R, Kremmer E, Hennige AM,
Hunder- Gugel A, et al. Insulin-induced serine phosphorylation of
IRS-2 via ERK1/2 and mTOR: studies on the function of Ser675 and
Ser907. Am J Physiol Endocrinol Metab. 2011; 300: E824-36.
28. Chen H, Michel T. Insulin signaling in vascular endothelial
cells: a key role for heterotrimeric G proteins revealed by
siRNA-mediated Gbeta1 knockdown. Biochemistry. 2006; 45:
29. Pramojanee SN, Phimphilai M, Chattipakorn N, Chattipakorn
SC. Possible roles of insulin signaling in osteoblasts. Endocr Res.
2014; 39: 144-51.
30. Yoon H, Kim HL, Chun YS, Shin DH, Lee KH, Shin CS, et al.
NAA10 controls osteoblast differentiation and bone formation as a
feedback regulator of Runx2. Nat Commun. 2014; 5: 5176.
31. Fujita T, Azuma Y, Fukuyama R, Hattori Y, Yoshida C, Koida
M, et al. Runx2 induces osteoblast and chondrocyte differentiation
and enhances their migration by coupling with PI3K-Akt signaling. J
Cell Biol. 2004; 166: 85-95.
32. Menon S, Dibble CC, Talbott G, Hoxhaj G, Valvezan AJ,
Takahashi H, et al. Spatial control of the TSC complex integrates
insulin and nutrient regulation of mTORC1 at the lysosome. Cell.
2014; 156: 771-85.
33. Fukumoto S, Martin TJ. Bone as an endocrine organ. Trends
Endocrinol Metab. 2009; 20: 230-6.
34. Zigdon-Giladi H, Bick T, Morgan EF, Lewinson D, Machtei EE.
Peripheral blood-derived endothelial progenitor cells enhance
vertical bone formation. Clin Implant Dent Relat Res. 2015; 17:
35. Fuchs S, Ghanaati S, Orth C, Barbeck M, Kolbe M, Hofmann A,
et al. Contribution of outgrowth endothelial cells from human
peripheral blood on in vivo vascularization of bone tissue
engineered constructs based on starch polycaprolactone scaffolds.
Biomaterials. 2009; 30: 526-34.
36. Sengupta A, Patel PA, Yuldasheva NY, Mughal RS, Galloway S,
Viswambharan H, et al. Endothelial insulin receptor restoration
rescues vascular function in male insulin receptor
haploinsufficient mice. Endocrinology. 2018; 159: 2917-25.
37. Chisalita SI, Arnqvist HJ. Insulin-like growth factor I
receptors are more abundant than insulin receptors in human micro-
and macrovascular endothelial cells. Am J Physiol Endocrinol Metab.
2004; 286: E896-901.
38. Tsuruzoe K, Emkey R, Kriauciunas KM, Ueki K, Kahn CR.
Insulin receptor substrate 3 (IRS-3) and IRS-4 impair IRS-1- and
IRS-2-mediated signaling. Mol Cell Biol. 2001; 21: 26-38.
39. LeRoith D, Werner H, Beitner-Johnson D, Roberts CT, Jr.
Molecular and cellular aspects of the insulin-like growth factor I
receptor. Endocr Rev. 1995; 16: 143-63.
40. Jacobo SM, Kazlauskas A. Insulin-like growth factor 1
(IGF-1) stabilizes nascent blood vessels. J Biol Chem. 2015; 290:
41. Sukhanov S, Higashi Y, Shai SY, Vaughn C, Mohler J, Li Y, et
al. IGF-1 reduces inflammatory responses, suppresses oxidative
stress, and decreases atherosclerosis progression in ApoE-deficient
mice. Arterioscler Thromb Vasc Biol. 2007; 27: 2684-90.
42. Huang B, Wang W, Li Q, Wang Z, Yan B, Zhang Z, et al.
Osteoblasts secrete Cxcl9 to regulate angiogenesis in bone. Nat
Commun. 2016; 7: 13885.
43. Ishida K, Matsumoto T, Sasaki K, Mifune Y, Tei K, Kubo S, et
al. Bone regeneration properties of granulocyte colony-stimulating
factor via neovascularization and osteogenesis. Tissue Eng Part A.
2010; 16: 3271-84.
44. Jose MV, Thomas V, Johnson KT, Dean DR, Nyairo E. Aligned
PLGA/HA nanofibrous nanocomposite scaffolds for bone tissue
engineering. Acta Biomater. 2009; 5: 305-15.
45. Mir M, Ahmed N, Rehman AU. Recent applications of PLGA based
nanostructures in drug delivery. Colloids Surf B Biointerfaces.
2017; 159: 217-31.
46. Wang X, Qi F, Xing H, Zhang X, Lu C, Zheng J, et al.
Uniform-sized insulin- loaded PLGA microspheres for improved
early-stage peri-implant bone regeneration. Drug Deliv. 2019; 26:
47. Wang F, Song YL, Li CX, Li DH, Zhang HP, Ma AJ, et al.
Sustained release of insulin-like growth factor-1 from
poly(lactide-co-glycolide) microspheres improves osseointegration
of dental implants in type 2 diabetic rats. Eur J Pharmacol. 2010;
48. Wang X, Wu X, Xing H, Zhang G, Shi Q, E L, et al. Porous
nanohydroxyapatite/collagen scaffolds loading insulin PLGA
particles for restoration of critical size bone defect. ACS Appl
Mater Interfaces. 2017; 9: 11380-91.
49. Zamani F, Amani-Tehran M, Latifi M, Shokrgozar MA. The
influence of surface nanoroughness of electrospun PLGA nanofibrous
scaffold on nerve cell adhesion and proliferation. J Mater Sci
Mater Med. 2013; 24: 1551-60.
50. Wang X, Zhang G, Qi F, Cheng Y, Lu X, Wang L, et al.
Enhanced bone regeneration using an insulin-loaded
nano-hydroxyapatite/collagen/PLGA composite scaffold. Int J
Nanomedicine. 2018; 13: 117-27.
51. Choi GH, Lee HJ, Lee SC. Titanium-adhesive polymer
nanoparticles as a surface-releasing system of dual osteogenic
growth factors. Macromol Biosci. 2014; 14: 496-507.
52. Ko E, Yang K, Shin J, Cho SW. Polydopamine-assisted
osteoinductive peptide immobilization of polymer scaffolds for
enhanced bone regeneration by human adipose-derived stem cells.
Biomacromolecules. 2013; 14: 3202-13.
53. Lee H, Dellatore SM, Miller WM, Messersmith PB.
Mussel-inspired surface chemistry for multifunctional coatings.
Science. 2007; 318: 426-30.
54. Liu M, Zeng G, Wang K, Wan Q, Tao L, Zhang X, et al. Recent
developments in polydopamine: an emerging soft matter for surface
modification and biomedical applications. Nanoscale. 2016; 8:
55. Gao T, Zhang N, Wang Z, Wang Y, Liu Y, Ito Y, et al.
Biodegradable microcarriers of poly(lactide-co-glycolide) and
nano-hydroxyapatite decorated with IGF-1 via polydopamine coating
for enhancing cell proliferation and osteogenic differentiation.
Macromol Biosci. 2015; 15: 1070-80.
56. Naik A, Shepherd DV, Shepherd JH, Best SM, Cameron RE. The
effect of the type of HA on the degradation of PLGA/HA composites.
Mater Sci Eng C Mater Biol Appl. 2017; 70: 824-31.
Nanotheranostics 2020, Vol. 4
57. van de Weert M, Hennink WE, Jiskoot W. Protein instability
in poly(lactic-co-glycolic acid) microparticles. Pharm Res. 2000;
58. Ngiam M, Liao S, Patil AJ, Cheng Z, Chan CK, Ramakrishna S.
The fabrication of nano-hydroxyapatite on PLGA and PLGA/collagen
nanofibrous composite scaffolds and their effects in osteoblastic
behavior for bone tissue engineering. Bone. 2009; 45: 4-16.
59. Simionescu BC, Drobota M, Timpu D, Vasiliu T, Constantinescu
CA, Rebleanu D, et al.
functionalized nano-hydroxyapatite hybrid cryogel: Synthesis,
characterization and application in gene delivery. Mater Sci Eng C
Mater Biol Appl. 2017; 81: 167-76.
60. Paul W, Nesamony J, Sharma CP. Delivery of insulin from
hydroxyapatite ceramic microspheres: preliminary in vivo studies. J
Biomed Mater Res. 2002; 61: 660-2.
61. Zhang Y, Zhang L, Ban Q, Li J, Li CH, Guan YQ. Preparation
and characterization of hydroxyapatite nanoparticles carrying
insulin and gallic acid for insulin oral delivery. Nanomedicine.
2018; 14: 353-64.
62. Yu W, Jiang G, Liu D, Li L, Tong Z, Yao J, et al.
Transdermal delivery of insulin with bioceramic composite
microneedles fabricated by gelatin and hydroxyapatite. Mater Sci
Eng C Mater Biol Appl. 2017; 73: 425-8.
63. Nandi SK, Kundu B, Mukherjee J, Mahato A, Datta S, Balla VK.
Converted marine coral hydroxyapatite implants with growth factors:
in vivo bone regeneration. Mater Sci Eng C Mater Biol Appl. 2015;
64. Haider A, Gupta KC, Kang IK. PLGA/nHA hybrid nanofiber
scaffold as a nanocargo carrier of insulin for accelerating bone
tissue regeneration. Nanoscale Res Lett. 2014; 9: 314.
65. Lasgorceix M, Costa AM, Mavropoulos E, Sader M, Calasans M,
Tanaka MN, et al. In vitro and in vivo evaluation of silicated
hydroxyapatite and impact of insulin adsorption. J Mater Sci Mater
Med. 2014; 25: 2383-93.
66. Scudeller LA, Mavropoulos E, Tanaka MN, Costa AM, Braga CAC,
Lopez EO, et al. Effects on insulin adsorption due to zinc and
strontium substitution in hydroxyapatite. Mater Sci Eng C Mater
Biol Appl. 2017; 79: 802-11.
67. Young S, Wong M, Tabata Y, Mikos AG. Gelatin as a delivery
vehicle for the controlled release of bioactive molecules. J
Control Release. 2005; 109: 256-74.
68. Liang HC, Chang WH, Lin KJ, Sung HW. Genipin-crosslinked
gelatin microspheres as a drug carrier for intramuscular
administration: in vitro and in vivo studies. J Biomed Mater Res A.
2003; 65: 271-82.
69. Chen FM, Zhao YM, Wu H, Deng ZH, Wang QT, Zhou W, et al.
Enhancement of periodontal tissue regeneration by locally
controlled delivery of insulin-like growth factor-I from
dextran-co-gelatin microspheres. J Control Release. 2006; 114:
70. Kim K, Lam J, Lu S, Spicer PP, Lueckgen A, Tabata Y, et al.
Osteochondral tissue regeneration using a bilayered composite
hydrogel with modulating dual growth factor release kinetics in a
rabbit model. J Control Release. 2013; 168: 166-78.
71. Madihally SV, Matthew HWT. Porous chitosan scaffolds for
tissue engineering. Biomaterials. 1999; 20: 1133-42.
72. Jayasuriya AC, Kibbe S. Rapid biomineralization of chitosan
microparticles to apply in bone regeneration. J Mater Sci Mater
Med. 2010; 21: 393-8.
73. Nandi SK, Kundu B, Basu D. Protein growth factors loaded
highly porous chitosan scaffold: a comparison of bone healing
properties. Mater Sci Eng C Mater Biol Appl. 2013; 33: 1267-75.
74. Mantripragada VP, Jayasuriya AC. IGF-1 release kinetics from
chitosan microparticles fabricated using environmentally benign
conditions. Mater Sci Eng C Mater Biol Appl. 2014; 42: 506-16.
75. Kim S, Kang Y, Krueger CA, Sen M, Holcomb JB, Chen D, et al.
Sequential delivery of BMP-2 and IGF-1 using a chitosan gel with
gelatin microspheres enhances early osteoblastic differentiation.
Acta Biomater. 2012; 8: 1768-77.
76. Larsen BE, Bjornstad J, Pettersen EO, Tonnesen HH, Melvik
JE. Rheological characterization of an injectable alginate gel
system. BMC Biotechnol. 2015; 15: 29.
77. Perteghella S, Martella E, de Girolamo L, Perucca Orfei C,
Pierini M, Fumagalli V, et al. Fabrication of innovative
silk/alginate microcarriers for mesenchymal stem cell delivery and
tissue regeneration. Int J Mol Sci. 2017; 18: 1829.
78. Goswami S, Bajpai J, Bajpai AK. Calcium alginate
nanocarriers as possible vehicles for oral delivery of insulin. J
Exp Nanosci. 2014; 9: 337-56.
79. Duruel T, Cakmak AS, Akman A, Nohutcu RM, Gumusderelioglu M.
Sequential IGF-1 and BMP-6 releasing chitosan/alginate/PLGA hybrid
scaffolds for periodontal regeneration. Int J Biol Macromol. 2017;
80. Cardoso AP, Goncalves RM, Antunes JC, Pinto ML, Pinto AT,
Castro F, et al. An interferon-gamma-delivery system based on
chitosan/poly(gamma- glutamic acid) polyelectrolyte complexes
modulates macrophage-derived stimulation of cancer cell invasion in
vitro. Acta Biomater. 2015; 23: 157-71.
81. Yan S, Rao S, Zhu J, Wang Z, Zhang Y, Duan Y, et al.
Nanoporous multilayer poly(L-glutamic acid)/chitosan microcapsules
for drug delivery. Int J Pharm. 2012; 427: 443-51.
82. Lin Y-H, Mi F-L, Chen C-T, Chang W-C, Peng S-F, Liang H-F,
et al. Preparation and characterization of nanoparticles shelled
with chitosan for oral insulin delivery. Biomacromolecules. 2007;
83. Hsieh CY, Tsai SP, Wang DM, Chang YN, Hsieh HJ. Preparation
of gamma- PGA/chitosan composite tissue engineering matrices.
Biomaterials. 2005; 26: 5617-23.
84. Shu X, Shi Q, Feng J, Xie X, Chen Y. Design and in vitro
evaluation of novel γ-PGA/hydroxyapatite nanocomposites for bone
tissue engineering. J Mater Sci. 2014; 49: 7742-9.
85. Shu X, Feng J, Feng J, Huang X, Li L, Shi Q. Combined
delivery of bone morphogenetic protein-2 and insulin-like growth
factor-1 from nano-poly (gamma-glutamic acid)/beta-tricalcium
phosphate-based calcium phosphate cement and its effect on bone
regeneration in vitro. J Biomater Appl. 2017; 32: 547-60.
86. Teotia AK, Gupta A, Raina DB, Lidgren L, Kumar A.
Gelatin-modified bone substitute with bioactive molecules enhance
cellular interactions and bone regeneration. ACS Appl Mater
Interfaces. 2016; 8: 10775-87.
87. Zimmermann G, Moghaddam A. Allograft bone matrix versus
synthetic bone graft substitutes. Injury. 2011; 42 Suppl 2:
88. Lei Y, Xu Z, Ke Q, Yin W, Chen Y, Zhang C, et al. Strontium
hydroxyapatite/chitosan nanohybrid scaffolds with enhanced
osteo-inductivity for bone tissue engineering. Mater Sci Eng C
Mater Biol Appl. 2017; 72: 134-42.
89. Ruixin L, Cheng X, Yingjie L, Hao L, Caihong S, Weihua S, et
al. Degradation behavior and compatibility of micro,
nanoHA/chitosan scaffolds with interconnected spherical macropores.
Int J Biol Macromol. 2017; 103: 385-94.
90. Maher SA, Doty SB, Torzilli PA, Thornton S, Lowman AM,
Thomas JD, et al. Nondegradable hydrogels for the treatment of
focal cartilage defects. J Biomed Mater Res A. 2007; 83:
91. Maleki H, Shahbazi MA, Montes S, Hosseini SH, Eskandari MR,
Zaunschirm S, et al. Mechanically strong silica-silk fibroin
bioaerogel: a hybrid scaffold with ordered honeycomb
micromorphology and multiscale porosity for bone regeneration. ACS
Appl Mater Interfaces. 2019; 11: 17256-69.
92. Li Y, Liu C. Nanomaterial-based bone regeneration.
Nanoscale. 2017; 9: 4862-74.
93. Wang B, Guo Y, Chen X, Zeng C, Hu Q, Yin W, et al.
Nanoparticle-modified chitosan-agarose-gelatin scaffold for
sustained release of SDF-1 and BMP-2. Int J Nanomedicine. 2018; 13:
94. Li L, Zhou G, Wang Y, Yang G, Ding S, Zhou S. Controlled
dual delivery of BMP-2 and dexamethasone by nanoparticle-embedded
electrospun nanofibers for the efficient repair of critical-sized
rat calvarial defect. Biomaterials. 2015; 37: 218-29.
95. Holland TA, Tabata Y, Mikos AG. Dual growth factor delivery
from degradable oligo(poly(ethylene glycol) fumarate) hydrogel
scaffolds for cartilage tissue engineering. J Control Release.
2005; 101: 111-25.
96. Kinard LA, Kasper FK, Mikos AG. Synthesis of
oligo(poly(ethylene glycol) fumarate). Nat Protoc. 2012; 7:
97. Chen FM, Chen R, Wang XJ, Sun HH, Wu ZF. In vitro cellular
responses to scaffolds containing two microencapulated growth
factors. Biomaterials. 2009; 30: 5215-24.
98. Malafaya PB, Oliveira JT, Reis RL. The effect of
insulin-loaded chitosan particle-aggregated scaffolds in
chondrogenic differentiation. Tissue Eng Part A. 2010; 16: